## 1 Introduction
SiC was added by a constant volume percent of 2 vol.%, while graphite was incorporated by different volume percentages at 2, 4, 6, 8, and 10 vol.%. These additive reinforcing materials will improve mechanical characteristics such as micro-hardness and compressive strength. The manufactured hybrid nanocomposites were produced by powder technology under applied pressure at 430 MPa, while the sintering process was carried out in an electrical furnace at 550 \({}^{\circ}\)C under an argon atmosphere to prevent the oxidation of the specimens. The results of this work show that the reinforcement materials were homogeneously dispersed in the aluminum matrix, which in turn improved the mechanical characteristics [22]. [PERSON] et al. manufactured the hybrid nanocomposites Al/Fe\({}_{3}\)O\({}_{4}\)/SiC via the powder technology method. This investigation has studied the effect of Fe\({}_{3}\)O\({}_{4}\) and SiC on their physical and mechanical properties. Fe\({}_{3}\)O\({}_{4}\) was incorporated by 15 wt.% and 30 wt.%, while SiC was added by a constant percent of 20 wt.%. Magnesium stearate was added as an activator material to prevent the accumulation of the reinforcement nanomaterials during the mixing process. SEM photomicrographs show that Fe\({}_{3}\)O\({}_{4}\) and SiC are homogeneously distributed into the aluminum matrix. The preferred density and micro-hardness for Al/30 wt.% Fe\({}_{3}\)O\({}_{4}\)/20 wt.% SiC after the sintering process were 2.69 g/cm\({}^{3}\) and 91 HV, respectively. Moreover, the wear rate decreased from 0.601 to 0.412 and the corrosion resistance from 90.91% to 99.83%, respectively [23]. [PERSON] and [PERSON] have produced aluminum reinforced by graphene nanosheets using powder technology. Graphene nanosheets were introduced into the aluminum matrix by 0.25 wt.%, 0.5 wt.% and 1.0 wt.%. The effect of graphene nanosheets on microstructure and mechanical properties was investigated. The results of scanning electron microscopy (SEM), X-ray diffraction (XRD), and transmission electron microscopy (TEM) examinations show a homogeneous dispersion of graphene nanosheets into the aluminum matrix. Additionally, XRD examination shows that the Al\({}_{4}\)C\({}_{3}\) phase was created at the interfaces between graphene nanosheets and aluminum atoms. Also, the results show an improvement in mechanical properties such as micro hardness, yield strength, and tensile strength with the addition of graphene nanosheets. This study emphasizes that the referred portion of graphene nanosheets is 0.25 wt.% [24]. [PERSON] et al. studied the physical properties, mechanical properties, and microstructure of aluminum nanocomposite manufactured by powder metallurgy. Nickel ferrite (NiFe\({}_{2}\)O\({}_{4}\)) nanoparticles at 35 nm have been incorporated at different percents (0 wt.%, 1 wt.%, 2.5 wt.%, 5 wt.%, and 10 wt.%). The mechanical and magnetic properties of the manufactured nanocomposites were defined. The microstructural analysis for the manufactured nanocomposites was conducted by FESEM, XRD, and DSC examinations, while the magnetic properties were defined by VSM examination. The results of this investigation show that the increasing weight percent (5 wt.%) of NiFe\({}_{2}\)O\({}_{4}\) ceramic nanoparticles will increase yield strength, tensile strength, and micro-hardness. FESEM images show a homogeneous dispersion of NiFe\({}_{2}\)O\({}_{4}\) ceramic nanoparticles into the aluminum matrix and then improve the density of nanocomposites for green compacts and sintered specimens. Moreover, increasing NiFe\({}_{2}\)O\({}_{4}\) to 0 wt.% will increase the magnetization, and compressive strength and decrease the elongation of the produced nanocomposite specimens [25]. [PERSON] et al. studied the friction and wear behavior of the aluminum alloy AA360 reinforced with SiC, B\({}_{4}\)C, and SiC/B\({}_{4}\)C particles using the pressured infiltration method. Dry sliding wear behavior was carried out by a pin-on-disc machine under applied loads of 10, 20, and 30 N and sliding speeds of about 0.5, 1.0, and 1.5 ms\({}^{-1}\).